Access the full text.

Sign up today, get DeepDyve free for 14 days.

Wigger, Daniel; Schmidt, Robert; Del Pozo-Zamudio, Osvaldo; Preuß, Johann A.; Tonndorf, Philipp; Schneider, Robert; Steeger, Paul; Kern, Johannes; Khodaei, Yashar; Sperling, Jaroslaw; de Vasconcellos, Steffen Michaelis; Bratschitsch, Rudolf; Kuhn, Tilmann

Condensed Matter
, Volume 2019 (1903) – Mar 27, 2019

/lp/arxiv-cornell-university/phonon-assisted-emission-and-absorption-of-individual-color-centers-in-NedsODYuT5

- ISSN
- 2053-1583
- eISSN
- ARCH-3331
- DOI
- 10.1088/2053-1583/ab1188
- Publisher site
- See Article on Publisher Site

Phonon-assisted emission and absorption of individual color centers in hexagonal boron nitride 1 2 Daniel Wigger , Robert Schmidt , Osvaldo Del 2;3 2 2 Pozo-Zamudio , Johann A. Preuß , Philipp Tonndorf , 2 2 2 Robert Schneider , Paul Steeger , Johannes Kern , Yashar 4 4 Khodaei , Jaroslaw Sperling , Steﬀen Michaelis de 2 2 1 Vasconcellos , Rudolf Bratschitsch and Tilmann Kuhn Institute of Solid State Theory, University of Münster, 48149 Münster, Germany Institute of Physics and Center for Nanotechnology, University of Münster, 48149 Münster, Germany Instituto de Investigación en Comunicación Optica, Universidad Autónoma de San Luis Potosí, 78210 San Luis Potosi, México Terahertz Technology and Photonics, Hübner GmbH & Co K.G., 34123 Kassel, Germany E-mail: d.wigger@wwu.de Abstract. Defect centers in hexagonal boron nitride represent room-temperature single-photon sources in a layered van der Waals material. These light emitters appear with a wide range of transition energies ranging over the entire visible spectrum, which renders the identiﬁcation of the underlying atomic structure challenging. In addition to their eminent properties as quantum light emitters, the coupling to phonons is remarkable. Their photoluminescence exhibits signiﬁcant side band emission well separated from the zero phonon line (ZPL) and an asymmetric broadening of the ZPL itself. In this combined theoretical and experimental study we show that the phonon side bands can be well described in terms of the coupling to bulk longitudinal optical (LO) phonons. To describe the ZPL asymmetry we show that in addition to the coupling to longitudinal acoustic (LA) phonons also the coupling to local mode oscillations of the defect center with respect to the entire host crystal has to be considered. By studying the inﬂuence of the emitter’s wave function dimensions on the phonon side bands we ﬁnd reasonable values for size of the wave function and the deformation potentials. We perform photoluminescence excitation measurements to demonstrate that the excitation of the emitters is most eﬃcient by LO-phonon assisted absorption. arXiv:1903.11295v1 [cond-mat.mes-hall] 27 Mar 2019 Phonon coupling in hBN color centers 2 1. Introduction Single-photon emitters are at the heart of many promising quantum technologies such as quantum computing and quantum cryptography. Although there are various solid-state emitters of single photons, there is still no system available, which simultaneously meets all requirements [1]. For example, self-assembled semiconductor quantum dots [2, 3] represent a mature technology platform, but presently yield optimum performance only at cryogenic temperatures. Another class of single-photon emitters are defect centers in insulators, such as color centers in diamond [4, 5, 6]. These defect centers exhibit prominent single-photon emission also at room temperature but suﬀer from a high refractive index and challenging processability of the host crystal. Recently, a new class of single-photon emitters in atomically thin semiconductors has been discovered [7, 8, 9, 10, 11, 12, 13] and has been deterministically positioned on the nanoscale by strain engineering [14, 15, 16]. Defect centers in hexagonal boron-nitride (hBN) combine features from these classes [17, 18, 19, 20, 21, 22, 23, 24, 25, 26, 27, 28, 8, 30, 31, 32]. They have the characteristics of an atomically sized defect center and at the same time share the advantages of a layered structure, i.e., the ultimate limit of miniaturization due to their atomic thickness and high mechanical robustness. In this work, we investigate the photoluminescence (PL) and photon absorption of defect centers in hBN nanocrystals. By developing a theoretical model to calculate the PL spectrum taking into account the coupling to bulk longitudinal optical (LO) and longitudinal acoustic (LA) phonons and to the oscillation of a local mode, we explain measured emission spectra achieving an excellent agreement between experiment and theory. In addition, we verify by means of photoluminescence excitation (PLE) spectroscopy that coupling to LO phonons provides an eﬃcient way of exciting individual single-photon emitters. This then allows for the isolation of a desired single-photon emitter from the wide range of emission energies of various defect centers in hBN. 2. Results 2.1. Emission spectra Localized single-photon emitters are investigated in hBN nanopowder deposited on a Si/SiO substrate (see Supplementary Material for details about the structure). Figure 1 presents typical measured room-temperature PL spectra of six diﬀerent localized light emitters in hBN. The transition energy of the emitters E , which is called the zero ZPL phonon line (ZPL) (labeled with numbers (1) to (6) in Fig. 1(a)) varies over a large range between 1.6 eV and 2.5 eV [19]. The energy of the excited states of the emitters has already been extensively studied, both theoretically via DFT calculations [33, 34, 35, 31] and experimentally [19, 23, 24, 25, 26, 27, 8, 31, 32, 36]. Although diﬀerent types of atomic defects such as N- or B-vacancies or substitutions with carbon or oxygen might exist, the distribution of transition energies is remarkably homogeneous. Therefore, it is unlikely that each emission energy in hBN stems from a diﬀerent type of defect. One Phonon coupling in hBN color centers 3 promising proposal for the measured wide range of transition energies is that at least part of the energy spread is due to a Stark shift [31] resulting from an electric ﬁeld which arises from a trapped charge near the color center [23]. Another suggested origin is a local strain distribution in the crystal [37, 28, 30, 36]. Our results suggest that both eﬀects might contribute to the broad energy spread of the ZPL energies. The narrow ZPLs of the emitters are accompanied by characteristic phonon side bands at lower energies. To compare the phonon side bands of the diﬀerent emitters more easily, the spectra are plotted against the detuning from the ZPL energy in Fig. 1(b). Two side bands well separated from the ZPL between 0.2 eV and 0.15 eV below E ZPL are visible, which can be attributed to two longitudinal optical (LO) phonons [21]. Also the ZPL itself is always more or less asymmetric with a steeper high energy side, which hints towards the contribution of low-energy (LE) phonon modes with energies below 50 meV. As will be shown later, we also assume two types of LE modes to be important. Comparing the phonon side bands of the diﬀerent emitters in Fig. 1(b) we ﬁnd signiﬁcant variations. Not only the relative height of the LO phonon side bands compared to the ZPL intensity, but also the detailed structure, i.e., the relative heights of the LO and LO peak with respect to each other, vary from emitter to emitter. Having a closer look at the LE phonon modes near the ZPL, also this spectral phonon feature has diﬀerent shapes and strengths for diﬀerent emitters as highlighted in Fig. 1(b). In the following sections we will study these phonon side bands and develop a detailed understanding of their origin. In this context we will discuss which arguments support the identiﬁcation of the LE phonons as longitudinal acoustic (LA) phonons and local mode oscillations of the defect with respect to the entire crystal. 2.2. Phenomenological analysis The properties of the LE and LO phonon side bands change signiﬁcantly among the emitters. Therefore, we ﬁrst try gaining a broad, quantitative overview of the diﬀerent features. For this purpose we use a phenomenological model to ﬁt the room temperature PL spectra of 165 diﬀerent emitters. Figure 1(c) shows an exemplary spectrum (blue) and its phenomenological ﬁt (orange). It is obvious that two LO phonon modes with energies at E 165 meV and E 195 meV have to be taken into account LO;1 LO;2 (red line). These energies are also supported by Raman measurements and ab initio calculations [1]. While trying diﬀerent models for the LE phonons we found that at least two LE modes are required to achieve reasonable ﬁts for all measured spectra. The best agreement was found for E = 14 meV and E = 30 meV. We will later LE LE 1 2 show that these energies can be well identiﬁed as representative for LA phonons in the case of LE and for a local mode in the case of LE . But for now we will stick to the 1 2 label LE phonons for the low energy side bands. The applied ﬁt function for the PL intensity reads I (E) = I (E) + I (E) + I (E) ; ZPL LO LE Phonon coupling in hBN color centers 4 (6) (5) (4) (3) (2) (1) 1.4 1.6 1.8 2 2.2 2.4 energy E (eV) LE LE LO LO × 3 (1) (2) (3) (4) (5) (6) −0.25 −0.2 −0.15 −0.1 −0.05 0 0.05 energy E − E (eV) ZPL exp. LE ﬁt LE abs ZPL LE abs LO LE 2 phonon 1.85 1.9 1.95 2 2.05 2.1 2.15 energy E (eV) Figure 1. Photoluminescence spectra. (a) Exemplary room temperature photoluminescence (PL) spectra with diﬀerent ZPL energies (1)–(6). (b) Same as (a) but plotted as a function of the detuning with respect to the ZPL energy to highlight the diﬀerent shapes of the phonon side bands. (c) Phenomenological ﬁt (orange) of a measured PL spectrum (blue). The constituents of the ﬁt are the ZPL (green), single phonon LO side bands (red), the low energy (LE) side bands LE (yellow) and LE 1 2 (violet) with the respective absorption peaks (dotted) and the two phonon side bands (dashed turquoise). where we include a ZPL, single-phonon processes for the LO phonons and single- and two-phonon processes for the LE phonons. We also take single-phonon absorption processes for the LE modes into account. For all peaks we assume a Lorentzian shape. normal. PL intens. normal. PL intens. normal. PL intens. Phonon coupling in hBN color centers 5 From each ﬁt we retrieve the integrated peak weights A (j = ZPL, LO , LO , LE , j 1 2 1 LE ) and respective peak widths (k = ZPL, LE , LE ), where we assume that the 2 k 1 2 LO side bands have the same broadening as the ZPL, which is a good approximation for dispersionless LO modes. Details about the ﬁt function can be found in the Supplementary Material. In Fig. 1(c) we additionally show the two LE side bands (yellow for LE and violet for LE ) in phonon emission (solid) and absorption (dotted). The 1 2 dashed turquoise line depicts the contribution from two phonon processes. Note that the absorption and two-phonon side bands are strictly related to the corresponding single- phonon emission side bands and therefore do not introduce additional ﬁt parameters. The ﬁt slightly deviates from the measurement for energies larger than the ZPL energy. The reason is, that a longpass ﬁlter is used close to the transition energy to block the exciting laser. This often reduces the measured high energy side of the ZPL. Therefore, we only used energies smaller than E for the ﬁts. ZPL For the large data set of 165 emitters we identify correlations between the diﬀerent spectral features. We start by comparing the LO phonon side bands to the ZPL. For this purpose, Fig. 2(a) shows the LO contribution, i.e., the ratio A =A LO ZPL (A = A + A ) between the LO side band and the ZPL weight, as a function of LO LO LO 1 2 the ZPL energy. The colors of the dots represent the energy of the driving laser. The photon energies of the three lasers are marked by the dashed lines. We ﬁnd transition energies almost equally distributed between 1.6 eV and 2.2 eV [22, 23, 25, 28, 36]. Even a few emitters appear above 2.4 eV. Larger transition energies could not be measured, because of the longpass ﬁlter blocking the exciting laser. Having a look at the values of the LO contribution, i.e., the vertical distribution of the dots, we ﬁnd that they have a clear tendency following a positive slope. While for transition energies below 1.9 eV most of the points lie between 0 and 0.2, they appear between 0.1 and 0.45 for energies around 2.1 eV. This shows that the emitters with smaller transition energies couple on average less eﬃciently to the optical phonons. This is in good agreement with the assumption that the shift of the ZPL energy is associated with the Stark eﬀect. A static electric ﬁeld acting on the emitter’s dipole should increase the distance between the diﬀerent charge centers. In consequence this should also inﬂuence the coupling to the polar LO phonons. The additional spread of LO side band strengths for a ﬁxed energy, especially around 2.1 eV, could be due to the eﬀect of local strain. Distortions of the lattice constants in the vicinity of the defect center should not only inﬂuence the distance between the charge centers, but also change the size of the emitter’s wave function and therefore the eﬀective distance between the charge centers. Later on we will discuss the inﬂuence of these properties on the phonon coupling in more detail. To shed more light on the properties of the LO phonons, Fig. 2(b) shows the energies of the LO phonon side bands as a function of the ZPL energy. We ﬁnd two clusters of data points, which we associate to the two LO phonon modes near the point. The energies of LO (yellow) appear around 165 meV, those of LO (violet) around 195 meV, 1 2 which agrees well with calculated band structures and Raman measurements [1]. As indicated by the dotted lines, we ﬁnd that the phonon energies have a slight trend to Phonon coupling in hBN color centers 6 1.2 0.22 LO E = 1.96 eV 1 L b LO 2.33 eV 0.21 2.76 eV 0.2 laser exc. 0.8 0.19 0.6 0.18 0.17 0.4 0.16 0.2 0.15 0 0.14 1.5 1.7 1.9 2.1 2.3 2.5 2.7 1.5 1.7 1.9 2.1 2.3 2.5 ZPL energy E (eV) ZPL energy E (eV) ZPL ZPL 1.2 1 25 0.5 c d 0.8 20 0.4 0.8 0.6 15 0.3 0.6 0.4 10 0.2 0.4 0.2 5 0.1 0.2 0 0 0 0 1.5 1.7 1.9 2.1 2.3 2.5 1.5 1.7 1.9 2.1 2.3 2.5 ZPL energy E (eV) ZPL energy E (eV) ZPL ZPL Figure 2. Correlations of diﬀerent phonon features. (a) LO phonon side band ratio A =A with the diﬀerent dot colors indicating the excitation energy marked LO ZPL by the dashed lines. (b) Energy separation of the LO phonon side bands from the ZPL, LO in yellow and LO in violet. A constant error of 0.01 eV is assumed because 1 2 these values are ﬁxed by hand for every spectrum. (c) LE phonon side band fraction A =A . The dot colors and sizes represent the contribution of LE to the entire LE ZPL 1 LE side band. (d) Width of the ZPL with the dot colors and sizes representing the LO side band fraction A =A from (a). LO ZPL higher values for larger ZPL energies. As we identify these energies with the phonon energies of the hBN bulk crystal, this correlation suggests that the origin of the energy shift of the ZPL should also inﬂuence the LO phonon energies. This could be the case for a local strain ﬁeld, which naturally changes the phonon dispersion. But also the dielectric environment might alter the LO phonon energies, as it aﬀects in particular the LO-TO splitting [39]. Figure 2(c) focusses on the LE phonon side bands by plotting the ratio between the ﬁrst side band weight A and the ZPL weight A as a function of the ZPL LE ZPL energy. The dots are scattered over a wide range from 0 to almost 1 for any transition energy. However, the majority of the points is equally distributed between 0.1 and 0.7. This ﬁnding does not provide any strong correlation between the coupling to the LE A /A A /A LE ZPL LO ZPL A /A LE LE ZPL width (meV) LO energies (eV) A /A LO ZPL Phonon coupling in hBN color centers 7 (LA) phonons and the transition energy. The color and size of the dots represents the LE contribution to the entire LE side band, i.e., A =A , where A = A + A 1 LE LE LE LE LE 1 1 2 (small dots are blue, large dots red). Also this quantity shows no correlation in the dot pattern. Small blue and large red dots are found everywhere. This suggests that the coupling to LE phonons is not strongly aﬀected by the parameters that are expected to govern the transition energy, i.e., the distance of the charge centers. However, we ﬁnd a wide spread of dots on the vertical axis, i.e., a non-negligible variation of coupling strengths for a given transition energy. This ﬁnding will be traced back to variations of the emitter’s size as discussed in more detail later. Finally, Fig. 2(d) presents the ZPL width as a function of ZPL energy. We ﬁnd a slight trend to smaller line widths at small transition energies, which is a similar to what has been found in Fig. 2(a) for the strength of the LO side bands. This is in line with established models which associate the ZPL width with second-order phonon coupling mechanisms [40]. The mechanism suggested in Ref. [40] relies on the scattering of acoustic phonons with the polaron formed by optical phonons. Consequently, a weaker coupling to LO phonons should result in a smaller lattice displacement of the polaron and therefore in a smaller scattering rate for the acoustic phonons. This could lead to the narrowing of the ZPL we found here. Another reason for this trend could be a stronger spectral wandering induced by trapped charges which are also considered as the origin of the Stark shift of the ZPL energies [23]. 2.3. Theoretical model The phenomenological model used to ﬁt the 165 spectra in Sec. 2.2 already includes some assumptions about the expected phonon modes, but it does not allow to retrieve further information about the emitters themselves. To support our assumptions about the mode energies we use a microscopically motivated model to reproduce the measured PL spectra. We also use this model to ﬁnd possible origins for the correlations and non-correlations of the diﬀerent phonon features and the ZPL energy found in Fig. 2. As already discussed in detail, our model should include the coupling to LO phonons to reproduce the two side bands around 165 meV and 195 meV below the ZPL. Also the coupling to acoustic phonons, which typically leads to a low-energy broadening of the ZPL, should be present in these systems. From defect centers in diamond, such as the extensively investigated NV center, it is well known that the prominent phonon side band is dominated by the coupling to local mode oscillations [41, 42]. These modes describe displacements of the defect atoms with respect to the entire host crystal. Due to the similarity of the atomic defect structures, we expect that also in hBN local modes might have a signiﬁcant inﬂuence on the PL spectrum. We model the PL intensity spectrum of an emitter by calculating the optical susceptibility for a two-level system coupled to phonons, which in the time domain Phonon coupling in hBN color centers 8 is given by [43, 44, 45, 46] (t) = i(t) exp i! t + (t) ; (1) where (t) denotes the Heaviside step function, ~! = E is the polaron-shifted 0 ZPL transition energy of the emitter, i.e., the energy of the zero phonon line, T the dephasing time and describes the phonon-induced dephasing with h i J (! ) ~! j ph ph (t) = coth cos(! t)1 i sin(! t) d! :(2) ph ph ph ! 2k T ph This phonon inﬂuence is determined by the temperature T and the phonon spectral density J at the phonon energy ~! for the phonon mode j. Note that such a model j ph was commonly used to simulate the phonon coupling of F-centers [43]. In this section T = 300 K is considered to allow comparison with the experimental results in Sec. 2.2. In the case of coupling to bulk phonons the spectral density is given by [47] J (! ) = jg (q)j [! ! (q)] : (3) j ph j ph j Here, g (q) denotes the coupling matrix element for the coupling to a phonon with wave vector q in the phonon branch j and ! (q) is the corresponding phonon dispersion relation. With Eq. (1) the absorption spectrum (!) of the emitter is simply given by the imaginary part of the Fourier transform 2 3 i!t 4 5 (!) = Im (t) e dt (4) From this expression the emission spectrum I (!) is then retrieved by inverting the absorption with respect to the ZPL at ! , i.e., I (!) = (! + 2! ) : (5) We account for the coupling of the defect to LO and LO phonons via the Fröhlich- 1 2 interaction h i e ! (q) 1 1 1 LO g (q) = F (q) F (q) (6a) LO e h 2" V ~ " (q) " (q) q 0 1 s and for the coupling to LA phonons via the deformation potential coupling h i g (q) = D F (q) D F (q) ; (6b) LA e e h h 2%~! (q)V LA where V is a normalization volume, % is the mass density, " and " are the static and s 1 high frequency dielectric functions, respectively, and D and D are the deformation e h potentials for electrons and holes, respectively. The form factors F (q) are determined e;h by the wave function of the excited state of the emitter as we explain in the following. Another common coupling mechanism between charges and LA phonons is via the piezoelectric eﬀect. In Ref. [48] it was shown that the piezoelectric constants vanish Phonon coupling in hBN color centers 9 with an increasing number of hBN layers. As we are investigating nanopowder samples, we are dealing with small bulk crystals with large layer numbers. The thickness of the investigated hBN crystals is continuously distributed between 40 nm and 100 nm as exemplarily shown in the Supplementary Material. In Ref. [48] it was demonstrated that due to inversion symmetry the piezoelectric constants vanish for even layer numbers. If this coupling mechanism to LA phonons played an important role, it should only appear for half of the studied defects, i.e., those located in samples with odd layer numbers. This eﬀect should lead to a separation of data points for crystals of even and odd layer number in Fig. 2(a) but one does not ﬁnd such a feature. Therefore, we conclude that the piezoelectric coupling to LA phonons does not play an important role in our samples and assume that this coupling mechanism can be neglected. One central aspect of hBN is its pronounced anisotropy arising from its layered structure. In our model we take this into account by distinguishing in-plane and out-of- plane directions. We assume that the dipole of the emitter lies in the plane of one hBN layer. Therefore, we consider a wave function of the defect’s excited state consisting of two diﬀerently charged centers with an in-plane distance d as schematically shown in Fig. 3(a). The negative charge will be referred to as electron (e) and the positive one as hole (h). Each of the charge centers has a Gaussian wave function with an in-plane localization length a and an out-of-plane localization length b. This form of the wave function can be seen as an approximation for a wave function typically calculated from ab initio theory. The advantage of our approach is the ﬂexibility to easily study the inﬂuence of changes of geometrical quantities. With this form of the wave function the form factors in Eqs. (6a) and (6b) read " # q a q b i r z F (q) = exp d q and (7a) 2 2 2 " # q a q b i r z F (q) = exp + d q ; (7b) 2 2 2 where the phonon wave vector q is split into an in-plane q and an out-of-plane q r z component and d is the vector connecting the two charge centers. After integrating jg (q)j in Eq. (3) over the in-plane angle of the phonon wave vector, the inﬂuence of the wave function geometry on the coupling strengths is given by h i h i 2 2 2 jg (q ; q )j exp (q a) + (q b) 1 J (dq ) (8a) LO r z r z 0 r and h i h i 2 2 2 2 2 jg (q ; q )j exp (q a) + (q b) D +D 2D D J (dq ) ; (8b) LA r z r z e h 0 r e h where J is the Bessel function of ﬁrst kind and of zeroth order. Due to these form factors, coupling to phonons is essentially restricted to the wave vector region q . a , q . b . For the Fröhlich coupling, diﬀerent dielectric constants for the in-plane and the out-of-plane direction are considered. The energies of the phonons, which enter the Phonon coupling in hBN color centers 10 LO LO TO LA ZO TA ZA A Γ M Figure 3. Model system. (a) Schematic drawing of the wave function of the defect in a single hBN layer. The charge centers have a Gaussian shape with an in-plane localization length a, an out-of plane localization length b and an in-plane distance d. (b) Phonon dispersion of hBN adapted from Ref. [1]. The A direction is the out-of-plane direction and the M direction an example for an in-plane direction. model, are extracted from the simulated dispersion relation shown in Fig. 3(b) adapted from Ref. [1]; we assume two LO modes (LO and LO ) with constant dispersions. For 1 2 the LA phonons we consider linear dispersions, where we again distinguish between the in-plane and the out-of-plane direction. More details about the model parameters can be found in the Supplementary Material. As will be shown below, the 14 meV LE mode introduced in Sec. 2.2 can be seen as a reasonable approximation for the side band stemming from the LA phonons. In Ref. [34] it was calculated that the C N center B V has the strongest coupling to an in-plane breathing mode of the defect center, which has an energy of 30 meV. Also other studies suggest this atomic structure as promising candidate for the hBN color center [49, 50]. This motivates us to interpret the LE mode in the phenomenological model in Sec. 2.2 as representative of such a breathing mode. The coupling to this local mode is modeled by a Lorentzian-like distribution of the phonon spectral density [51, 52, 53] 1 16g ! ! LOC ph J (! ) = : (9) LOC ph 2 2 2 ! ! + 4 ! LOC ph ph phonon energy (meV) Phonon coupling in hBN color centers 11 The parameters entering this coupling are the local mode energy ~! = E , the LOC LOC coupling strength g and the width . For the considered parameters the spectral shape of the side band due to the local mode agrees well with the ordinary Lorentzian shape considered for the phenomenological ﬁts in Sec. 2.2. We show in the Supplementary Material that our model for the local mode coupling reproduces PL spectra of diﬀerent defect centers in diamond very well, showing the accuracy of the model. To reproduce the ﬁnite width of the ZPL, we assume a constant dephasing rate 1=T , providing us with a dephasing time T . We note that this dephasing time includes pure dephasing, homogeneous broadening mechanisms as well as inhomogeneous processes, e.g., spectral wandering [27]. While the phonon dispersion relations and dielectric constants are well known for hBN, the deformation potentials are only hardly known. Simulations indicate that the relevant values are in the range of some hundred meV to a few eV [54]. We therefore will try ﬁnding reasonable values for the deformation potentials D and D for the LA e h phonon coupling of the considered defect centers in hBN. The other unknown parameters in our model are the in-plane and out-of-plane localization lengths a and b, respectively, and the charge separation d in the defect state. To be able to extract information on these parameters from the measured spectra, we will analyze their role for the coupling to LO and LA phonon modes, respectively. For the coupling to LO phonons the only unknown quantities are the geometrical parameters in-plane localization length a, out-of-plane localization length b, and charge distance d. To investigate their inﬂuence, we ﬁrst concentrate on the coupling to LO phonons. In Fig. 4(a) we plot the contribution of the LO single-phonon side band, i.e., the fraction between the weight of the ﬁrst LO phonon side bands of LO and LO and 1 2 the ZPL weight, as a function of the charge distance d for diﬀerent localization lengths a between 0.1 nm (blue) and 1 nm (red). The distance d is varied on the same scale. This should be a reasonable range for these quantities as the in-plane lattice constant of hBN is 0.4 nm and the extension of an atomistic defect state should be of similar size. Under the assumption that the Stark eﬀect is responsible for the diﬀerent transition energies of the emitters, we additionally plot the measured data points from 2(a) as gray dots into Figs. 4(a). The relation between the energies of the experimental values of Fig. 2(a) (gray dots in Fig. 4(a)) and the charge distances d in Fig. 4(a) is obtained by the ﬁts of the measured spectra in Sec. 2.4, which yield values between d = 0:2 nm and d = 0:5 nm. By the given choice of the ZPL energy axis the majority of the measurement points appear in this range. The simulated LO contributions vanish for vanishing in-plane distance d because in this limit there is no dipole moment associated with the defect. For a given in-plane localization length a the LO contribution grows with increasing d. When increasing the localization length a the curves rise slower, because the Fröhlich coupling strength depends on the eﬀective dipole strength of the wave function. To achieve the same strength for larger localization lengths a the charge separation has to be accordingly larger. The increase of the LO contribution with increasing distance nicely resembles the distribution of the measured dot pattern, which Phonon coupling in hBN color centers 12 measured ZPL energy (eV) 1.5 1.7 1.9 2.1 2.3 2.5 2.7 2.5 2 a = 0.1 nm exp. 1.5 a = 0.1 nm d = 1.2 nm 0.6 nm 0.3 nm LO 0.15 nm LO +LO 1 2 0.1 nm 0.5 2LO 2LO 2 1 LO a = 0.5 nm a = 1 nm 0 0.2 0.4 0.6 0.8 1 −0.4 −0.3 −0.2 −0.1 0 charge dist. d (nm) energy E − E (eV) ZPL 1 1 sim. w/ LA phon. c d d phenom. ﬁt | D − D | = e h 1 eV ZPL 0.75 eV LE 0.5 eV LE 0.25 eV 0 eV abs LE 0 1 2 abs | D − D | (eV) LE e h T = 0.17 ps a = 0.4 nm b = 0.2 nm d = 0 nm 0 0 −60 −40 −20 0 20 40 −0.1 −0.05 0 0.05 0.1 energy E − E (eV) ZPL energy E − E (meV) ZPL Figure 4. (a) Contribution of the ﬁrst LO phonon side band with respect to the ZPL A =A as a function of the charge distance d for diﬀerent localization lengths LO ZPL a. The gray dots are the measurements from Fig. 2(a). (b) Exemplary simulated normalized PL spectra for diﬀerent d from large (bright) to small values (dark), for a = 0:1 nm (top) and a = 0:5 nm (bottom). (c) Exemplary simulated normalized PL spectra for diﬀerent values of jD D j and vanishing charge separation. Inset: e h LA phonon contribution as a function of deformation potential diﬀerence jD D j. e h (d) Phenomenological ﬁt of a simulated PL spectrum including the coupling to LA phonons. supports the interpretation that the shift of the ZPL is at least partially related to a Stark shift. To further analyze the inﬂuence of the LO phonons, we show exemplary normalized PL spectra for diﬀerent values of a and d in Fig. 4(b). The colors agree with the corresponding curves in (a). At the bottom for a = 0:5 nm the two single-phonon LO side bands are well resolved around 0:2 eV, also the three two-phonon side bands between 0:3 eV and 0:4 eV can be seen. As expected the amplitude of the side bands increases for larger in-plane distance d. At the top of Fig. 4(b) the same spectra are LO contribution A /A LO ZPL normal. PL intensity LA contr. normal. PL intensity normal. PL intens. Phonon coupling in hBN color centers 13 shown for a = 0:1 nm. Here, the LO side bands grow very rapidly when increasing d, they even become larger than the ZPL. For the largest considered d the two-phonon side bands are even larger than the single-phonon side bands. Indeed, from Eqs. (2) and (3) it can be shown that, as long as successive side bands do not spectrally overlap, the contributions of single-phonon (A ) and two-phonon (A ) side bands with respect LO 2LO to the ZPL are given by 2 2 g (q) A A 1 A LO LO j 2LO LO = ; = : (10) A ! A 2 A ZPL LO ZPL ZPL j;q Thus, as soon as A > 2A the two-phonon sideband will exceed the single-phonon LO ZPL one. However, in the measured PL spectra of hBN color centers this regime where the side bands exceed the ZPL is not reached. Therefore, we can conclude that the localization length should lie between a = 0:3 nm and 1 nm and the charge distance between d = 0 nm and 1 nm. After ﬁnding reasonable values for the in-plane size of the wave function (a and d), in Figs. 4(c) we focus on the values for the deformation potentials D and D . When e h considering the special case of a vanishing charge distance, d = 0, the deformation potential coupling strength in Eq. (8b) is proportional to (D D ) . So we will use e h this limit to ﬁnd reasonable values for the diﬀerence of the deformation potentials. To provide a quantitative measure, we calculate the LA contribution to the entire spectrum via h i 1 Im (t ! 1; ! = 0; T ! 1) : (11) LA 0 2 This value is plotted as a function of jD D j in the inset in Fig. 4(c) for wave function e h dimensions of a = 0:4 nm, b = 0:2 nm and d = 0 nm. For D = D the LA contribution e h vanishes and no LA side band appears in the spectrum, while the side band dominates the entire spectrum for large values of jD D j. In Fig. 2(c) we found that the LA e h contribution in the measured spectra also for small transition energies, i.e., small d, yields values between zero and one. Therefore, reasonable values for the diﬀerence of the deformation potentials should lead to an LA contribution of around 0.5. We ﬁnd that this is fulﬁlled for jD D j 0:6 eV. However, the deformation potentials not only e h determine the LA contribution but are also responsible for the shape of the spectra. To demonstrate this inﬂuence, we show exemplary spectra for diﬀerent values of jD D j e h still for a vanishing dipole moment d = 0 in Fig. 4(c). We ﬁnd that with increasing jD D j (blue to red) the asymmetry of the ZPL peak increases till the entire spectrum e h is dominated by the LA side band for the 1 eV case (red). Here the ZPL is only a rather small peak on the broad phonon background. From here on we ﬁx jD D j = 0:6 eV. e h As already mentioned, we assume that the coupling to the LE mode phenomenologically describes the coupling to LA phonons. One might wonder why the coupling to a discrete mode with a Lorentzian lineshape approximates reasonably well the coupling to the continuum of LA phonons. To conﬁrm that this is indeed a valid approximation, the black solid line in Fig. 4(d) shows a simulated room-temperature Phonon coupling in hBN color centers 14 PL spectrum, where the coupling to the continuum of LA phonons is fully taken into account. This spectrum was then ﬁtted by the phenomenological model of Sec. 2.2 yielding the orange line. The contributions of the two LE modes (yellow and violet) and the ZPL (green) in the phenomenological model are plotted separately as before. We ﬁnd an excellent agreement between the simulated spectrum including only LA phonons and the phenomenological ﬁt. Furthermore we ﬁnd that only the LE mode has a relevant contribution in the ﬁt. This shows that indeed the LE mode is a reasonable approximation for the contribution of the LA phonons to the spectrum. In the next step we investigate the inﬂuence of the sum of the deformation potentials. For a non-vanishing charge distance d the Bessel function in Eq. (8b) does not vanish leading to the fact that the phonon coupling depends on D and D separately. In e h Fig. 5(a) we show simulated PL spectra for a = 0:4 nm, b = 0:2 nm and d = 0:5 nm and diﬀerent values of D +D between 0 eV (blue) and 1 eV (red). We ﬁnd that the weight of e h the LA side bands close to the ZPL strongly increases with the sum of the deformation potentials. It is also nicely visible that the LO phonon side bands are additionally broadened by the LA phonons, demonstrating that multi-phonon contributions are well reproduced by the model. In Fig. 2(c) we found that the LA contribution (LE mode) to the spectrum exhibits no signiﬁcant correlation with the transition energy, i.e., with d. This ﬁnding should be reproduced by the choice of D + D . Therefore, in Fig. 5(b) e h we plot the LA contribution as a function of the charge distance d for diﬀerent values of D + D between 0 eV (blue) and 4 eV(red) (a = 0:4 nm and b = 0:2 nm). All curves e h start at the same value of slightly below 0.6 for d = 0 nm. We ﬁnd that for deformation potential sums of 1 eV or larger the LA contribution grows signiﬁcantly with increasing d. One would therefore expect a clear correlation between these two quantities. This makes us conclude that D + D should be smaller than 1 eV. In the special case of e h D + D = 0:6 eV = jD D j the LA contribution is a straight line, because in e h e h this case either D = 0 eV or D = 0 eV, which makes the charge distance irrelevant. h e However, we do not expect one of the deformation potentials, either for electrons or for holes, to vanish in hBN. This would mean that either electrons or holes do not scatter with LA phonons via the deformation potential coupling, which makes us disregard this value. We found good results for D + D = 0:2 eV (D = 0:4 eV, D = 0:2 eV) as e h e h will be demonstrated below in Sec. 2.4 when directly comparing the simulations with measured PL spectra. After having selected reasonable values for the deformation potentials, we now study the inﬂuence of the other two geometrical parameters, the in-plane localization length a and the out-of-plane localization length b of the wave function. Figures 5(c,d) focus on the in-plane localization length a. In Fig. 5(c) exemplary spectra for d = 0:5 nm, b = 0:2 nm and diﬀerent values of a between 0.2 nm (blue) and 1 nm (red) are shown. While the LO phonon side bands increase signiﬁcantly when reducing a, as discussed earlier, the LA phonon side band next to the ZPL does not change signiﬁcantly. To provide a quantitative measure for the inﬂuence of a on the LA coupling in Fig. 5(d) we plot the LA contribution as a function of a for diﬀerent values of d. All curves slightly Phonon coupling in hBN color centers 15 1 1 a b b b |D − D | = 0.6 eV e h D + D = 4 eV e h 0.9 D + D = 4 eV e h 3 eV 3 eV 2 eV 2 eV 1 eV a = 0.4 nm 0.8 1 eV 0 eV b = 0.2 nm 0.6 eV 0.2 eV d = 0.5 nm 0.7 0 eV 0.6 0 0.5 −0.4 −0.3 −0.2 −0.1 0 0 0.2 0.4 0.6 0.8 1 energy E − E (eV) charge distance d (nm) ZPL 1 1 D = 0.4 eV c d d a = 0.2 nm D = −0.2 eV 0.8 0.4 nm b = 0.2 nm 0.6 nm d = 0.5 nm 0.8 nm 0.6 1 nm d = 0.1 nm 0.4 0.3 nm 0.5 nm 0.2 0.7 nm 0.9 nm 0 0 −0.4 −0.3 −0.2 −0.1 0 0 0.2 0.4 0.6 0.8 1 energy E − E (eV) localization length a (nm) ZPL 1 1 e D = 0.4 eV a = 0.2 nm e f b = 0.2 nm D = −0.2 eV 0.4 nm 0.4 nm 0.8 0.6 nm a = 0.4 nm 0.6 nm 0.8 nm d = 0.5 nm 0.8 nm 1 nm 0.6 1 nm 0.4 LO LO 0.2 LO LO LA contr. 0 0 −0.4 −0.3 −0.2 −0.1 0 0 0.2 0.4 0.6 0.8 1 energy E − E (eV) localization length b (nm) ZPL Figure 5. Inﬂuence of (a,b) deformation potentials D + D and charge separation e h d, (c,d) in-plane localization length a and (e,f) out-of-plane localization length b on the spectra. (a,c,e) Exemplary normalized PL spectra. (b,d,e) LA contribution as functions of the wave function dimensions d, a and b. (f) also shows the fraction of the LO single-phonon side band peak intensities. decrease from values between 0.6 and 0.7 to 0.4 for a = 1 nm. This spread can give rise to part of the spread of LA contributions found in Fig. 2(c). Finally, the inﬂuence of the out-of-plane localization length b is considered. In Fig. 5(e) we again show PL spectra for a = 0:4 nm, d = 0:5 nm and diﬀerent values of b between 0.2 nm (blue) and 1 nm (red). Two pronounced features are found in the spectra: (i) the LA phonon side band increases with decreasing b; (ii) the two LO normal. PL intesnity normal. PL intesnity normal. PL intesnity LO LA contrib. or LA contribution LA contribution LO 1 Phonon coupling in hBN color centers 16 single-phonon side bands LO and LO slightly increase with decreasing b, but not by 1 2 the same rate. While LO and LO are almost equally strong for b = 1 nm (red), LO is 1 2 1 signiﬁcantly stronger for 0.2 nm (blue). These two features are quantiﬁed in Fig. 5(f). The solid lines show the LA contribution and the dashed lines the ratio between the peak intensities of the two LO single-phonon side bands I =I as functions of b LO LO 2 1 for diﬀerent values of a. The LA contribution rapidly drops from values up to 0.9 for b = 0 nm to 0.2 for b = 1 nm. This spread of LA phonon side band contributions agrees well with the measured values found in Fig. 2(c). The fraction of the LO side band peaks increases for growing b. This variation of the shape of the LO side band was also found in the measured spectra in Fig. 1. The reason for this variation of the LO side bands is that the larger LO phonon energy is not present for the out-of-plane phonon wave vectors, as can be seen in Fig. 3(b). So b mainly inﬂuences the LO phonon side band. A larger out-of-plane localization length b in Eq. (8a) leads to a smaller range of out-of-plane phonon wave vectors that is excited by the emitter, which leads to a weaker eﬀective coupling strength. Therefore the fraction I =I reduces for growing b. The LO LO 2 1 out-of-plane lattice constant of hBN is 0.66 nm, which makes the considered values for b a reasonable range for this parameter. This parameter study shows that slight variations of the geometrical parameters of the defect’s wave function in the range of reasonable dimensions lead to strong changes in the PL spectra. In the next step, we apply this model to directly reproduce measured PL spectra by varying the geometrical parameters. We also take the local mode for the low-energy coupling in the range of 30 meV into account and vary its coupling parameters. 2.4. Comparison between experiment and theory Figure 6 shows PL measurements of diﬀerent defect centers. While the spectra in Figs. 6(a,b) are taken at room temperature, Figs. 6(c,d) are measured at cryogenic temperatures of about 7 K. Figure 6(e) depicts a temperature series taken on the same emitter. The temperature decreases from top to bottom from 300 K to 20 K. In addition to the experiments (colored lines) we show corresponding simulations as black lines. All parameters for the simulations are listed in Tab. 1. Comparing the diﬀerent spectra, we ﬁnd a convincing agreement between the measured and the calculated spectra. The theoretical approach used in Ref. [24], which considers the phonon spectral function as a free parameter, also led to good agreements with measured spectra. However, the authors did not draw conclusions on the emitters’ wave functions and details of the electron-phonon coupling matrix elements. From the parameters for the dimensions of the wave functions in our model listed in Tab. 1 we ﬁnd that all sizes (a, b, and d) are in the range between 0.1 nm and 0.5 nm. This is a reasonable parameter range, because it shows that the assumed emitter wave function spreads over a few unit cells at most and is mainly restricted to the layer in which the defect is located. While the LO phonon energies scatter slightly around the already Phonon coupling in hBN color centers 17 a T = 300 K e T = 300 K 0.5 180 K 100 K 20 K 7 K 0 simulation 1.8 1.9 2 2.1 2.2 b T = 300 K 0.5 1.9 2 2.1 2.2 2.3 0.5 c T = 7 K 1.8 1.9 2 0.5 d T = 7 K w/o local mode w/ local mode local LA LO mode LO 1.9 2 2.1 1.9 2 2.1 2.2 energy E (eV) energy E (eV) Figure 6. Reproducing measured PL spectra. Normalized measured (colored) and simulated (black) PL spectra. (a,b) room temperature 300 K, (c,d) cryogenic temperature 7 K. (e) Temperature series from 300 K to 20 K from top to bottom of the same emitter. The model parameters are given in Tab. 1. discussed values of E 165 meV and E 195 meV, the energy of the local LO LO 1 2 mode is rather ﬁxed. This might have two reasons. On the one hand, the side band in the PL spectrum partly overlaps with the LA contribution at room temperature, which makes a precise determination of the peak position less easy. On the other hand, strain distributions could have less inﬂuence on the energetic position of the mode, but rather change the coupling strength g and the width . We want to remark that, the low temperature spectrum in Fig. 6(d) shows a pronounced peak at E 2:05 eV, i.e., 35 meV below the ZPL. The dashed line includes this peak as a local mode in the simulation. However, this spectral feature could also stem from another nearby emitter. Usually, PL spectra at cryogenic temperatures exhibit a large number of narrow lines in these samples, which makes a clear identiﬁcation of the lines diﬃcult. normal. PL intensity Phonon coupling in hBN color centers 18 Table 1. Model parameters for the simulations in Fig. 6 including the temperature T , the localization lengths a and b, the charge distance d, the LO phonon energies E LO and E , and the local mode energy E and coupling strength g=! . The local LO LOC LOC mode width ~ and the dephasing time T depend on the temperature. Fig. 6 T a b d E E E g=! ~ T LO LO LOC LOC 2 1 2 (K) (nm) (nm) (nm) (meV) (meV) (meV) (meV) (ps) (a) 300 0.40 0.40 0.44 165 200.0 30 0.38 15 0.08 (b) 300 0.50 0.10 0.40 163 200.0 30 0.30 18 0.12 (c) 7 0.40 0.15 0.25 161 192.0 30 0.15 5.0 (0.8) (d) 7 0.20 0.40 0.22 161 198.0 (35) (0.35) (2.0) (0.8) (e) 300 0.25 0.30 0.30 165 200.5 30 0.21 15 0.17 150 7.0 0.33 50 4.0 (0.4) 20 2.5 (0.5) To reproduce the entire temperature series in Fig. 6(e) we ﬁx the dimensions of the wave function and the local mode coupling strength for T = 300 K as given in Tab. 1. For each temperature we have to additionally determine the local mode width and the dephasing time T . We ﬁnd that both the ZPL and the local mode side band, which remains as narrow peak slightly above E = 2:1 eV for T = 20 K, become narrower with lower temperatures. This can already be seen when comparing the room-temperature spectra in Figs. 6(a,b) to the low-T ones in Figs. 6(c,d). In the Supplementary Material we discuss another temperature series of PL spectra taken on a diﬀerent emitter, where we additionally measured the PL lifetime. In agreement with Ref. [22] we ﬁnd that the life time does not depend on the temperature and that it is in the range of a few nanoseconds [17, 18, 19, 21, 27, 36]. This indicates that the ZPL line width at room temperature is dominated by the pure dephasing mechanism and spectral wandering, which we combine in the ﬁt parameter of the dephasing time T . For decreasing temperatures, the ZPL width shrinks signiﬁcantly as also found in Refs. [20, 22]. However, the values for low temperatures between 5 K and 50 K are underestimated because the measured line width is on the order of the limited resolution of the spectrometer (100 μeV). Hence, we are not able to draw reliable conclusions about the low-temperature T times from our data. The evolution of the two low-energy phonon side bands with decreasing temperature nicely supports our assumptions of their nature. The local mode results in an isolated peak at the same energy. This is not expected for phonons with continuous spectrum, i.e., for LA modes. The LA phonons lead to a low-energy side band directly attached to the ZPL, as it is well known from semiconductor QDs [55]. In the spectra in Fig. 6(e) we ﬁnd that the spectral shape of the LO phonon side band is additionally broadened to the high energy side compared to the simulation. When moving from high to low T , all spectral features become narrower, 0.750.8 0.650.7 0.550.6 0.450.5 0.350.4 0.250.3 0.150.2 0.050.1 Phonon coupling in hBN color centers 19 which makes it obvious that this broadening evolves into another maximum just below E = 2 eV. The ﬁts for the low-temperature spectra in Figs. 6(c,d) show that our model reproduces the LO phonon side bands, despite our rough approximations for the phonon dispersion when assuming constant LO phonon energies. However, it was shown that strain strongly inﬂuences the emitters’ spectra [37, 28, 30] and that it is highly likely that the emitters appear near the surface of the sample [23, 19]. Local strain or the proximity to the surface will alter the phonon band structure and could thereby lead to variations of the spectral shape of the LO side bands. This could be a reason for the atypical broadening of the LO side band for this emitter. 2.5. Photoluminescence excitation spectra We now focus again on the distribution of ZPL energies in Fig. 2(a). We ﬁnd that many of the green dots cluster around E = 2:15 eV, while the red dots cluster around 1.8 eV. ZPL These energies are approximately 150–200 meV below the respective photon energy of the laser used for excitation (dashed lines), which is the range of LO phonon energies. This suggests that LO-phonon assisted absorption could eﬃciently drive the emitters. Therefore, we plot a histogram of detunings between the exciting laser energy E and the ZPL energy E in Fig. 7(a), where the colors correspond to the colors in Fig. 2(a). In ZPL total, nearly 50% of all 165 investigated emitters appear between 150 meV and 200 meV below the laser energy. The remaining emitters are almost equally distributed over the remaining 800 meV. This agrees with the ﬁndings in Ref. [26]. PLE(ZPL+LE) E = 1.96 eV a b PLE(LO) 2.33 eV PL 2.76 eV PL (mirrored) integration for PLE(ZPL+LE) integration for PLE(LO) – – – – – – – – 1.7 1.8 1.9 2 2.1 2.2 2.3 energy E (eV) detuning E − E (eV) L ZPL Figure 7. LO phonon assisted absorption. (a) Histogram of ZPL energies with respect to their detuning from the exciting laser. The colors mark the diﬀerent laser excitations from Fig. 2(a). (b) Photoluminescence excitation (PLE) data retrieved from the ZPL (blue solid line) and the LO sideband (yellow solid line). The room temperature PL spectrum is plotted in orange with the shaded areas marking the integration areas to retrieve the PLE signals. The mirrored PL spectrum is given in green. To conﬁrm that the emitters are eﬃciently excited by LO-phonon assisted absorption, we have performed PLE measurements at room temperature to obtain relative quantity (%) PLE/PL intensity (arb. u.) Phonon coupling in hBN color centers 20 information about the absorption properties of the emitters at diﬀerent photon energies. The results are shown in Fig. 7(b). We chose an emitter which has a strong LO phonon sideband in the PL spectrum, as shown with the orange line. At the high-energy side of the ZPL at 2.03 eV the spectrum is again cut oﬀ by a longpass ﬁlter. We measure PL spectra for a wide range of diﬀerent excitation energies from 2.09 eV to 2.3 eV as shown in the Supplementary Material. After ﬁtting and subtracting the background and Raman lines as described in the Supplementary Material, we extract the PLE data by integrating the PL spectra either over the ZPL, i.e., from 1.95 eV to 2.05 eV (blue shaded area), or over the LO phonon sideband, i.e., from 1.75 eV to 1.9 eV (yellow shaded area). The PLE data for the ZPL and for the LO phonon sideband are shown in blue and yellow, respectively. We ﬁnd that both PLE data sets exhibit a pronounced maximum between 2.2 eV and 2.3 eV. This energy range nicely agrees with the phonon sidebands of the mirrored PL spectrum (green line). This observation demonstrates that the excitation of the emitter is very eﬃcient via the LO-phonon assisted process. Our study shows that the LO-phonon assisted excitation of the excited defect state provides an optimized way to drive the system. Therefore we can conclude that it is conceivable that we select a speciﬁc ZPL energy ~! , when pumping the system with energies between ~! + 160 meV and ~! + 200 meV, i.e, via a LO-phonon assisted 0 0 absorption. This provides a strategy of isolating single-photon emitters with a desired emission energy from the wide range of possible transitions. 3. Conclusions We have shown that the coupling to diﬀerent phonon modes plays a crucial role for localized light emitters in hBN. On the one hand, coupling to bulk phonons leads to an asymmetric broadening of the ZPL in the case of LA modes and to the appearance of prominent sidebands well separated from the ZPL in the case of LO modes. On the other hand the coupling to a local mode oscillation contributes to the broadening of the ZPL at room temperature, while the respective side band is discernible at cryogenic temperatures. By ﬁtting measured PL spectra with our theoretical model we were able to extract parameters for the wave function geometries of the emitters. We have shown that the distance between the positive and the negative charge center may be connected to the energy of the ZPL, supporting the assignment of the ZPL energy spread with the Stark eﬀect caused by nearby charges. It was also possible to ﬁnd reasonable values for the deformation potential of electrons and holes in hBN. By measuring PLE spectra, we have demonstrated that these sidebands are also present in absorption and lead to an eﬃcient absorption via LO-phonon assisted transitions. Finally we have shown that it is possible to preferentially select emitters with a desired transition from the wide range of emission energies possible in hBN by aiming at the LO-phonon assisted absorption. Our results lead to a deeper understanding of the fundamental properties of color centers in hBN and pave the way to a tailored control of the excitation process. Phonon coupling in hBN color centers 21 Acknowledgments We gratefully acknowledge support by the research group FOR 1493 of the Deutsche Forschungsgemeinschaft. We thank Michael Rohlﬁng for fruitful discussions. References [1] Aharonovich I, Englund D and Toth M 2016 Nature Photon. 10 631–641 [2] Santori C, Pelton M, Solomon G, Dale Y and Yamamoto Y 2001 Phys. Rev. Lett. 86 1502 [3] edited by Peter Michler 2003 Single quantum dots: Fundamentals, applications and new concepts (Topics in Applied Physics) vol 90 (Springer Verlag, Berlin) [4] Zaitsev A M 2000 Phys. Rev. B 61 12909 [5] Jelezko F and Wrachtrup J 2006 Phys. Status Solidi A 203 3207–3225 [6] Beha K, Batalov A, Manson N B, Bratschitsch R and Leitenstorfer A 2012 Phys. Rev. Lett. 109 [7] Tonndorf P, Schmidt R, Schneider R, Kern J, Buscema M, Steele G A, Castellanos-Gomez A, van der Zant H S J, Michaelis de Vasconcellos S and Bratschitsch R 2015 Optica 2 347–352 [8] Koperski M, Nogajewski K, Arora A, Cherkez V, Mallet P, Veuillen J Y, Marcus J, Kossacki P and Potemski M 2015 Nature Nanotech. 10 503–506 [9] Srivastava A, Sidler M, Allain A V, Lembke D S, Kis A and Imamoğlu A 2015 Nature Nanotech. 10 491–496 [10] He Y M, Clark G, Schaibley J R, He Y, Chen M C, Wei Y J, Ding X, Zhang Q, Yao W, Xu X, Lu C Y and Pan J W 2015 Nature Nanotech. 10 497–502 [11] Chakraborty C, Kinnischtzke L, Goodfellow K M, Beams R and Vamivakas A N 2015 Nature Nanotech. 10 507–511 [12] Tonndorf P, Schwarz S, Kern J, Niehues I, Del Pozo-Zamudio O, Dmitriev A I, Bakhtinov A P, Borisenko D N, Kolesnikov N N, Tartakovskii A I, Michaelis de Vasconcellos S and Bratschitsch R 2017 2D Materials 4 021010 [13] Palacios-Berraquero C, Barbone M, Kara D M, Chen X, Goykhman I, Yoon D, Ott A K, Beitner J, Watanabe K, Taniguchi T, Ferrari A C and Atatüre M 2016 Nature Comm. 7 [14] Kern J, Niehues I, Tonndorf P, Schmidt R, Wigger D, Schneider R, Stiehm T, Michaelis de Vasconcellos S, Reiter D E, Kuhn T and Bratschitsch R 2016 Adv. Mater. 28 7101–7105 [15] Branny A, Kumar S, Proux R and Gerardot B D 2017 Nature Comm. 8 15053 [16] Palacios-Berraquero C, Kara D M, Montblanch A R P, Barbone M, Latawiec P, Yoon D, Ott A K, Loncar M, Ferrari A C and Atatüre M 2017 Nature Comm. 8 15093 [17] Tran T T, Bray K, Ford M J, Toth M and Aharonovich I 2016 Nature Nanotech. 11 37–41 [18] Tran T T, Zachreson C, Berhane A M, Bray K, Sandstrom R G, Li L H, Taniguchi T, Watanabe K, Aharonovich I and Toth M 2016 Phys. Rev. Appl. 5 034005 [19] Tran T T, Elbadawi C, Totonjian D, Lobo C J, Grosso G, Moon H, Englund D R, Ford M J, Aharonovich I and Toth M 2016 ACS Nano 10 7331–7338 [20] Vuong T Q P, Cassabois G, Valvin P, Ouerghi A, Chassagneux Y, Voisin C and Gil B 2016 Phys. Rev. Lett. 117 097402 [21] Martínez L J, Pelini T, Waselowski V, Maze J R, Gil B, Cassabois G and Jacques V 2016 Phys. Rev. B 94 121405 [22] Jungwirth N R, Calderon B, Ji Y, Spencer M G, Flatté M E and Fuchs G D 2016 Nano Lett. 16 6052–6057 [23] Shotan Z, Jayakumar H, Considine C R, Mackoit M, Fedder H, Wrachtrup J, Alkauskas A, Doherty M W, Menon V M and Meriles C A 2016 ACS Photonics 3 2490–2496 [24] Exarhos A L, Hopper D A, Grote R R, Alkauskas A and Bassett L C 2017 ACS nano 11 3328–3336 Phonon coupling in hBN color centers 22 [25] Li X, Shepard G D, Cupo A, Camporeale N, Shayan K, Luo Y, Meunier V and Strauf S 2017 ACS Nano 11 6652–6660 [26] Jungwirth N R and Fuchs G D 2017 Phys. Rev. Lett. 119 057401 [27] Sontheimer B, Braun M, Nikolay N, Sadzak N, Aharonovich I and Benson O 2017 Phys. Rev. B 96 121202 [28] Grosso G, Moon H, Lienhard B, Ali S, Efetov D K, Furchi M M, Jarillo-Herrero P, Ford M J, Aharonovich I and Englund D 2017 Nat. commun. 8 705 [29] Tran T T, Kianinia M, Nguyen M, Kim S, Xu Z Q, Kubanek A, Toth M and Aharonovich I 2017 ACS Photonics 5 295–300 [30] Chejanovsky N, Kim Y, Zappe A, Stuhlhofer B, Taniguchi T, Watanabe K, Dasari D, Finkler A, Smet J H and Wrachtrup J 2017 Sci. Rep. 7 14758 [31] Noh G, Choi D, Kim J H, Im D G, Kim Y H, Seo H and Lee J 2018 Nano Lett. 18 4710–4715 [32] Xu Z Q, Elbadawi C, Tran T T, Kianinia M, Li X, Liu D, Hoﬀman T B, Nguyen M, Kim S, Edgar J H, Wu X, Song L, Ali S, Ford M, Toth M and Aharonovich I 2018 Nanoscale 10 7957–7965 [33] Grinyaev S N, Konusov F V and Lopatin V V 2002 Phys. Solid State 44 286–293 [34] Tawﬁk S A, Ali S, Fronzi M, Kianinia M, Tran T T, Stampﬂ C, Aharonovich I, Toth M and Ford M J 2017 Nanoscale 9 13575–13582 [35] Abdi M, Chou J P, Gali A and Plenio M B 2018 ACS Nano 5 1967–1976 [36] Proscia N V, Shotan Z, Jayakumar H, Reddy P, Cohen C, Dollar M, Alkauskas A, Doherty M, Meriles C A and Menon V M 2018 Optica 5 1128–1134 [37] Bourrellier R, Amato M, Galv~ ao Tizei L H, Giorgetti C, Gloter A, Heggie M I, March K, Stéphan O, Reining L, Kociak M and Zobelli A 2014 ACS Photonics 1 857–862 [38] Serrano J, Bosak A, Arenal R, Krisch M, Watanabe K, Taniguchi T, Kanda H, Rubio A and Wirtz L 2007 Phys. Rev. Lett. 98 095503 [39] Sohier T, Gibertini M, Calandra M, Mauri F and Marzari N 2017 Nano Lett. 17 3758–3763 [40] Machnikowski P 2006 Phys. Rev. Lett. 96 140405 [41] Huxter V M, Oliver T A A, Budker D and Fleming G R 2013 Nature Phys. 9 744–749 [42] Kehayias P, Doherty M W, English D, Fischer R, Jarmola A, Jensen K, Leefer N, Hemmer P, Manson N B and Budker D 2013 Phys. Rev. B 88 165202 [43] Duke C B and Mahan G D 1965 Phys. Rev. 139 A1965 [44] Mahan G D 2013 Many-particle physics (Springer Science & Business Media) [45] Schmitt-Rink S, Miller D A B and Chemla D S 1987 Phys. Rev. B 35 8113 [46] Krummheuer B, Axt V M and Kuhn T 2002 Phys. Rev. B 65 195313 [47] Reiter D E, Kuhn T, Gl’assl M and Axt V M 2014 J. Phys. Condens. Matter 26 423203 [48] Michel K H and Verberck B 2011 Phys. Rev. B 83 115328 [49] Sajid A, Reimers J R and Ford M J 2018 Phys. Rev. B 97 064101 [50] López-Morales G I, Proscia N V, López G E, Meriles C A and Menon V M 2018 arXiv preprint arXiv:1811.05924 [51] Garg A, Onuchic J N and Ambegaokar V 1985 J. Chem. Phys. 83 4491–4503 [52] Thorwart M, Hartmann L, Goychuk I and Hänggi P 2000 J. Mod. Opt. 47 2905–2919 [53] Norambuena A, Reyes S A, Mejía-Lopéz J, Gali A and Maze J R 2016 Phys. Rev. B 94 134305 [54] Wiktor J and Pasquarello A 2016 Phys. Rev. B 94 245411 [55] Jakubczyk T, Delmonte V, Fischbach S, Wigger D, Reiter D E, Mermillod Q, Schnauber P, Kaganskiy A, Schulze J H, Strittmatter A, Langbein W, Kuhn T, Reitzenstein S and Kasprzak J 2016 ACS Photonics 3 2461–2466 Phonon coupling in hBN color centers 1 Supplementary Material 1. Experimental details 1.1. Sample preparation Single-photon emitters (SPE) in hexagonal boron nitride are observed in hBN nano- powder (Sigma-Aldrich, grain size <150 nm). The powder is micromechanically exfoliated using scotch tape and stamped onto a Silicon substrate with a 80 nm or 270 nm thick thermal oxide layer on top. Figure 1 shows exemplary images of the nano powder sample. Panels (a) and (b) show a reﬂectance and PL image of the same sample area, respectively. The dark spots in (a) are clusters of the hBN powder crystals. The PL map in (b) shows bright spots at the positions of the clusters, where each spot stems from one or more defect centers. The SEM image in (c) shows the detailed stacked disc-like structure of the individual hBN crystals. a b 10 µm 10 µm 0.5 µm Figure 1. (a) Reﬂectance and (b) photoluminescence (PL) image of hBN nano-powder exfoliated onto SiO2/Si substrate. (c) SEM image of hBN nano-powder. The shape of the hBN nano-powder (Sigma Aldrich) is disc-like with diameters ranging from tens to hundreds of nanometers. The thickness of the discs varies from several nanometers up to hundreds of nanometers. Reﬂected counts PL counts Phonon coupling in hBN color centers 2 1.2. Photoluminescence and photoluminescence excitation spectroscopy The photoluminescence experiments are carried out in a homebuilt confocal microscope. For excitation at 2.76 eV (450 nm) a diode laser and at 2.33 eV (532 nm) a frequency- doubled Nd:YAG laser is used. For recording the PLE spectra, the emitters are excited with a tunable laser light source based on a continuous-wave (cw) optical parametric oscillator (OPO). The turn-key system (from Hübner Photonics) covers the wavelength range of 450 nm – 650 nm (2.76 eV – 1.91 eV). For the room-temperature measurements, the laser is focussed to the diﬀraction limit by an objective lens (numerical aperture NA=0.9), resulting in a focus size of 400 nm. The excitation power is 100 μW and kept constant for all excitation energies. For the temperature-dependent measurements, the sample resides in a ﬂow-cryostat cooled by liquid Helium. In this experiment, the laser is focussed on the sample using an objective lens with a NA of 0.75. In both cases, the same objective lens is used to collect the photoluminescence of the single emitters and the PL is analyzed in a spectrometer with an attached liquid nitrogen-cooled CCD camera. A longpass ﬁlter at 2.06 eV is used to remove stray light of the laser from the PL signal. 2. Theory 2.1. Phenomenological model As explained in the main text we use a phenomenological ﬁt function to extract relative spectral contributions from the phonon side bands of 165 diﬀerent emitters. The full ﬁt function consists of three parts with I (E) = I (E) + I (E) + I (E) ; (12) ZPL LO LE where the zero phonon line (ZPL) is given by ZPL ZPL I (E) = : (13) ZPL 2 2 (E E ) + ZPL ZPL The longitudinal optical (LO) phonon side bands are assumed to have the same width as the ZPL, which leads to the function I (E) = I (E) + I (E) (14) LO LO LO 1 2 LO ZPL [E (E E )] + ZPL LO 1 ZPL LO ZPL + ; (15) 2 2 [E (E E )] + ZPL LO 2 ZPL where E are the LO phonon energies. LO 1;2 Because the considered low energy (LE) phonon contributions have energies of E = LE 14 meV and E = 30 meV they are in the range of the thermal energy at room LE temperature k T 25 meV. Therefore we take phonon emission (I (E)) and B LE abs absorption (I (E)) processes into account. Additionally we consider two phonon LE j Phonon coupling in hBN color centers 3 2ph processes (I (E)) for these modes and combination of LO and LE processes. Therefore, LE the LE phonon side bands read abs 2ph I (E) = I (E) + I (E) + I (E) ; (16) LE LE j LE LE j j j=1;2 The single LE phonon lines read LE LE j j I (E) = ; (17) LE 2 2 [E (E E )] + ZPL LE j LE LE LE j j j abs I (E) = ; (18) LE j 2 n + 1 [E (E + E )] + j ZPL LE LE where n is the thermal occupation of LE mode j from the Bose-Einstein distribution. to reduce the number of ﬁt parameters we assume that the weights of the two phonon processes scale like the single LE phonon processes. This leads to the ﬁt function h i 2ph LO k abs I (E) = I (E E ) + I (E E ) LE LO LO LE j k LE k j j ZPL k=1;2 h i LE k abs + I (E E ) + I (E E ) : (19) LE LE LE j k LE k ZPL 2.2. Model parameters Motivated by Ref. [1], for the LO phonon energies we consider two constant energies and for the LA phonons linear dispersions. We distinguish between the in-plane and the out-of-plane direction with ~! (q ) = E ; ~! (q ) = E ; ! (q ) = c q LO r LO LO r LO LA r r r 1 1 2 2 ~! (q ) = E ; ~! (q ) = E ; ! (q ) = c q LO z LO LO z LO LA z z z 1 1 2 1 The sound velocities are chosen to c = 3:44 nm/ps [2] for the out-of-plane direction and for the in-plane direction we consider the mean value of the two high symmetry directions with c = 16 nm/ps, which we extract from the dispersion relations in Ref. [3]. Also the dielectric constants are diﬀerent in the two distinct lattice directions with [4] " (q ) = 4:95 ; " (q ) = 7:04 ; 1 r s r " (q ) = 4:10 ; " (q ) = 5:09 1 z s z We interpolate between the two given directions via 2 2 ! (q) = cos (' )! (q ) + sin (' )! (q ) j q j r q j z 2 2 "(q) = cos (' )"(q ) + sin (' )"(q ) q r q z where ' = atan(q =q ) is the angle of q with respect to the hBN-plane. q z r Phonon coupling in hBN color centers 4 3. Temperature-dependent photoluminescence measurement To conﬁrm the conclusions from the temperature-dependent measurements drawn in the main text, in Fig. 2 we show a second data set for a diﬀerent localized emitter. a a = 0.25 nm b T = 300 K b = 0.15 nm 150 K 50 K d = 0.16 nm 5 K simulation g = 0 meV T = 0.08 ps T = 0.17 ps T = 2.29 ns T = 2.32 ns T = 0.59 ps 1 T = 2.24 ns T = 0.81 ps 1 1.7 1.75 1.8 1.85 1.9 1.95 2 2 - 0 2 4 6 8 10 12 14 energy E (eV) time t (ns) Figure 2. Temperature-dependent PL spectra of one localized emitter. The temperature decreases from top to bottom (red to blue). The simulation is shown in green. The temperatures T are given next to each spectrum. In Fig. 2(a) the measured PL spectra (color) are shown for decreasing temperatures from top to bottom. The corresponding simulations are shown as black lines. The parameters used are given in the plot next to each curve. Here only the dephasing time T is adjusted for each temperature, while the other parameters are kept constant. We did not ﬁnd strong indications for a contribution of the local mode, leading to a coupling strength of g = 0 in the simulations. The deformation potential couplings are the same as in the main text (D = 0:4 eV and D = 0:2 eV). We again ﬁnd that the ZPL e h strongly narrows when reducing the temperature. In addition we measured the lifetime of the PL signal for diﬀerent temperatures. These measurements are carried out in the same setup as the low-temperature PL measurements (see Sec. 1.2). However, the emitters are excited by a tunable femtosecond ﬁber laser system ( 250 fs pulse length, 40 MHz repetition rate) at an energy of 2:16 eV [5]. The photoluminescence is detected using a Picoquant PDM Series single-photon counting module (timing accuracy 50 ps) and the PL decay measurement is performed with a Becker & Hickl SPC-130-EM time-correlated single-photon counting normal. PL intensity Phonon coupling in hBN color centers 5 card. The excitation power is kept constant for all measurements at 150 μW. The results are shown in Fig. 2(b). We extract the lifetime T by ﬁtting the data with a convolution of the instrument response function and a single exponential decay (black curves). We ﬁnd that the lifetime is almost constant T 2:3 ns for all considered temperatures. These values are on the same time scale as those of defect centers in diamond [6]. In Refs. [7, 8] it was shown, that the homogenous linewidth of the emitters at low temperatures is in the sub-μeV range and the corresponding T in the ns range. In this case, the dephasing is dominated by the lifetime of the excited state, i.e., additional dephasing eﬀects such as spectral wandering or pure dephasing vanish. This supports our observed trend of a strong narrowing of the ZPL with decreasing temperature. However, the values for low temperatures (5 K and 50 K) are underestimated because the measured line width is on the order of the limited resolution of the spectrometer (100 μeV). Hence, we are not able to draw reliable conclusions about the low-temperature T times from our data. At room temperature, we ﬁnd that the radiative lifetime is four orders of magnitude longer than the dephasing time. Therefore, we can conclude that the dephasing due to the radiative lifetime is negligible compared to other dephasing mechanisms. Phonon coupling in hBN color centers 6 4. Color centers in diamond Figure 3 shows PL spectra of the nitrogen vacancy (NV ) and the H3 color center in diamond in orange, respectively. The single-crystal diamond plate used for this experiment has a lateral size of 3 3 mm and a thickness of 1 mm and is produced by a high-pressure, high-temperature process (element6) and contains approximately 200 ppm nitrogen. For the excitation of the NV center (H3-center) we used a 532 nm laser diode (405 nm laser diode) with a power of 100 μW at the sample position. The focus diameter is 1.2 μm for 532 nm excitation and 1.4 μm for 405 nm excitation. Both spectra were measured at cryogenic temperatures. The blue curves represent the calculated spectra, where the coupling to a single local mode was considered. The model parameters with the best agreement with the experiment are listed in Tab. 2. NV H3 C C N N V V simulation 1.5 1.6 1.7 1.8 1.9 2 2.1 2.2 2.3 2.4 2.5 energy E (eV) Figure 3. PL spectra of color centers in diamond. Measured PL intensity for the NV (orange) and the H3 defect (blue). Simulation in black. The insets show the atomic structures of the defects. Table 2. Model parameters for the simulations in Fig. 3. The table shows the defect type, the ZPL energy ~! , the emitter dephasing time T and the local mode energy 0 2 ~! , its strength g and its width ~. LOC defect ~! (eV) T (ps) ~! (meV) g=! ~ (meV) 0 2 LOC LOC NV 1.95 0.45 65.16 0.87 14.7 H3 2.47 0.95 40.8 0.82 7.5 normal. PL intensity Phonon coupling in hBN color centers 7 5. PLE measurements In Fig. 4(a) PL spectra for diﬀerent excitation energies are shown. The ZPL maxima and the phonon sidebands reside on a background signal. For excitation energies between 2.09 eV and 2.22 eV, Raman lines appear, which shift with the laser energy. The Raman shifts of the three lines are 63 meV, 118 meV, and 168 meV. We attributed the ﬁrst two to the Si substrate [9] and the third one to the LO energy [10]. To extract the intensity of the ZPL and the phonon sidebands, we ﬁt the background by an exponential multiplied by an error function to reproduce the edge of the ﬁlter. The Raman lines are modeled by Gaussians. The background- and Raman-line-corrected spectra are shown in Fig. 4(b). For small excitation energies around 2.1 eV, which are very close to the ZPL energy, The PL spectra are very weak. Therefore both PLE signals in Fig. 7 in the main text drop signiﬁcantly. This surprising observation indicates that in the energetic range where excitation processes - including the local mode - should occur, the emitter is not excited. Looking at the PL spectra in Fig. 4(a) we see that for small excitation energies the ZPL overlaps with a strong Raman line, which might spoil the evaluation of the PLE data. Apart from that, the deviation between the PLE spectrum and the mirrored emission spectrum remains unclear and deserves additional investigation which is however beyond the scope of this paper. a raw data b background corrected ZPL ZPL ﬁlter LO laser LO laser E = 2.29 eV E = 2.29 eV E = 2.09 eV E = 2.09 eV L L 1.8 1.9 2 2.1 2.2 2.3 1.8 1.9 2 2.1 2.2 2.3 Raman lines energy E (eV) energy E (eV) Figure 4. PL spectra for diﬀerent excitation energies. Low excitation energies at the bottom (E = 2:09 eV), high energies at the top (E = 2:29 eV) (blue to red). (a) Raw L L PL data. (b) Background- and Raman-line-corrected spectra. PL intensity PL intensity Phonon coupling in hBN color centers 8 References [1] Serrano J, Bosak A, Arenal R, Krisch M, Watanabe K, Taniguchi T, Kanda H, Rubio A and Wirtz L 2007 Phys. Rev. Lett. 98 095503 [2] Bosak A, Serrano J, Krisch M, Watanabe K, Taniguchi T and Kanda H 2006 Phys. Rev. B 73 [3] Michel K H and Verberck B 2009 Phys. Rev. B 80 224301 [4] Geick R, Perry C H and Rupprecht G 1966 Phys. Rev. 146 543 [5] Sotier F, Thomay T, Hanke T, Korger J, Mahapatra S, Frey A, Brunner K, Bratschitsch R and Leitenstorfer A 2009 Nature Phys. 5 352 [6] Batalov A, Zierl C, Gaebel T, Neumann P, Chan I Y, Balasubramanian G, Hemmer P R, Jelezko F and Wrachtrup J 2008 Phys. Rev. Lett. 100 077401 [7] Dietrich A, Bürk M, Steiger E S, Antoniuk L, Tran T T, Nguyen M, Aharonovich I, Jelezko F and Kubanek A 2017 arXiv:1712.06938 [8] Tran T T, Kianinia M, Nguyen M, Kim S, Xu Z Q, Kubanek A, Toth M and Aharonovich I 2017 ACS Photonics 5 295–300 [9] Uchinokura K, Sekine T and Matsuura E 1972 Solid State Commun. 11 47–49 [10] Reich S, Ferrari A C, Arenal R, Loiseau A, Bello I and Robertson J 2005 Phys. Rev. B 71 205201

Condensed Matter – arXiv (Cornell University)

**Published: ** Mar 27, 2019

Loading...

You can share this free article with as many people as you like with the url below! We hope you enjoy this feature!

Read and print from thousands of top scholarly journals.

System error. Please try again!

Already have an account? Log in

Bookmark this article. You can see your Bookmarks on your DeepDyve Library.

To save an article, **log in** first, or **sign up** for a DeepDyve account if you don’t already have one.

Copy and paste the desired citation format or use the link below to download a file formatted for EndNote

Access the full text.

Sign up today, get DeepDyve free for 14 days.

All DeepDyve websites use cookies to improve your online experience. They were placed on your computer when you launched this website. You can change your cookie settings through your browser.